- Original article
- Open Access
Detection of the effective refractive index of thermally modified Scots pine by immersion liquid method
© The Japan Wood Research Society 2012
- Received: 27 May 2011
- Accepted: 5 September 2011
- Published: 20 January 2012
The purpose of this study was to determine the effective refractive index of thermally modified Scots pine (Pinus sylvestris L.) wood specimens as a quantitative measure regarding the change of wood density which is due to the thermal modification. The refractive index of thermally modified Scots pine wood was obtained by introducing pine wood powder into an immersion liquid and measuring light backscattering with a homebuilt multifunction spectrophotometer. The present method provides useful information that in principle can be applied, for example, in the optimization of the thermal modification process and inspection of the quality of thermally modified wood.
- Immersion liquid method
- Refractive index
- Thermally modified pine
Thermal modification at a typical temperature of 180–220°C is an industrial treatment applied for almost 100,000 m3 of sawn timber in Finland annually (Thermowood® production statistics 2010) . Thermal modification of wood aims at improving wood’s resistance against mold and decay fungi, dimensional stability, weather resistance, and appearance [2–4]. The improved dimensional stability is derived from the decrease of the hydroxyl groups that increases the hydrophobicity of wood and reduces the absorption of water . This results in lowered equilibrium moisture content. A majority of the extractives is removed from the wood, and its porosity is increased as the treatment temperature and time increase . Furthermore, wood’s colour turns to brown throughout the cross section. There is a practical need for easy-to-use, inexpensive and rapid analysis method that could be applied for defining the treatment temperature from wood specimens after the thermal modification. This would help monitoring the quality of thermally modified wood in the markets.
Wood consists mainly of cellulose, hemicelluloses and lignin. Cellulose and hemicelluloses are polysaccharides while lignins are highly complex, mainly aromatic polymers of phenylpropane units. Wood also contains small amounts of extractives such as resin and fatty acids, fats, fatty alcohols, waxes, phenols, terpenes, and steroids . The crystalline cellulose contains long-chain polysaccharides composed of β-1,4-linked d-glucose rings that cause rotation of linearly polarized light, which results from the birefringence of uniaxial cellulose crystal . The extraordinary refractive index of cellulose n e is 1.5956 and the ordinary refractive index n 0 is 1.5312 and thus the positive birefringence is 0.0643 (concentration of water is zero) for the sodium D-line . In the literature, an estimate of 1.557 is given for the effective refractive index of cellulose . Since any wood has various constituents that have different refractive indices the refractive index obtained by measurement is a weighted average of the constituents, and it is called the effective refractive index.
A variety of measurement techniques for determining optical properties of wood material such as the refractive index and birefringence have been developed. These include, e.g., ellipsometry , interferometry , polarized light microscopy , reflectometry , X-ray diffraction , ultrasound , and terahertz techniques . Unfortunately, many of these measurement techniques require rather expensive devices and good specimen quality in terms of homogeneity and smoothness [17, 18].
The objective of this study was to investigate the refractive index of thermally modified Scots pine (Pinus sylvestris L.) wood by an immersion liquid method. The immersion method has been popular for determination of the refractive index of microscopic minerals, identification of unknown solids , and inspection of the heterogeneity of the cell population in microbiology . In addition, immersion method has been utilized in tissue measurements in medicine. Anisotropic minerals have been studied with the immersion method . Wood, which has a much more complicated structure than a mineral, has also anisotropy in its structure. The advantages of the immersion method are that it is independent of the shape and size of a particle, and the measurement is relatively easy and fast to perform . The principle of the immersion method is to match the refractive index of solid particles with that of the immersion liquid. In the event of a perfect match between the index of the light non-absorbing particles and the immersion liquid, the light transmittance will be 100% and the scattering intensity of light will be zero. However, in the presence of insoluble birefringent (double refraction of light) particles, which form a two-phase system with the immersion liquid, the light transmission measurement method usually fails in situations where the particle density is high and a relatively long optical path is required for the measurement of the transmittance. On the contrary, another type of measurement method that can be used for the detection of the effective refractive index of birefringent particles, namely the light backscattering measurement technique which was exploited in this study, is free from such problems.
In the previous studies we have used a homebuilt multifunction spectrophotometer (MFS) for the measurement of refractive index of liquids. Furthermore, the MFS has been useful for the measurement of the refractive index of isotropic, and also effective refractive index of anisotropic (birefringent) pigments by using the immersion liquid method [22–24]. The advantages of the MFS over conventional devices that are used for the refractive index measurement of particles are: (1) refractive indices of both the immersion liquid and the pigment can be estimated using only one device; (2) measurement can be done both in the light transmission or scattering mode; and (3) the probe wavelength can be freely chosen in the UV–visible spectral range.
In this study, the effective refractive index of thermally modified Scots pine wood was measured for different treatment temperatures. The effective refractive index is proportional to the porosity of the wood.
The thermal modification of the specimens was performed according to the Thermowood® process . Scots pine sawn timber with dimensions of 63 (R) × 75 (T) × 2000 (L) mm were treated at 180, 200 and 230°C with actual heat treatment time of 3 h in the maximum temperature. The boards were sawn from trees that had grown in Central Finland, approximately between 64–65°N and 27–28°E. The boards contained both heartwood and sapwood.
In reality, it is usually difficult to adjust the measurement direction of the optical properties of wood with respect to an “optic axis” of a macroscopic wood specimen because the orientation of wood grains changes as a function of the thickness of the specimen. For instance, the birefringence of cellulose of wood is therefore usually detected from a fibre. In our study, the thermally modified boards were cut into approximately 5 × 5 × 5 mm pieces using a band saw. These pieces were ground in a refiner (CYCLOTEC 1093 Sample Mill) with 1.0-mm diameter circular holes. Finally, the powder obtained was dried at 103°C for 24 h and then put into a glass tube with cork closed for restoration. The higher thermal modification temperatures resulted in finer powders compared to the lower temperatures.
Measurement results for the density, effective refractive index and loss of birefringence of thermally modified Scots pine
Effective refractive index
Change of effective refractive index
Relative change of effective refractive index (%)
Based on Fig. 2, we can notice that the minimum level of the backscattering signal decreases in the vertical direction when the treatment temperature rises. Nevertheless, the BS is always higher than zero. This indicates that thermally modified Scots pine contains constituents that have different refractive indices. One such a constituent is the birefringent cellulose, and one explanation we propose as the reason for lowering of the minimum value of BS is the loss of birefringence of the cellulose due to crystal to amorphous deformation . Thermal modifications of crystalline structure of cellulose of beech and spruce were studied in . In that study, the cellulose was isolated and using KBr (alkali halide) disks to collect Fourier transform infrared (FT-IR) spectra. Our study is different from  because we studied Scots pine and did not use KBr matrix.
In our study, the untreated specimens had the highest BS, whereas the lowest BS was obtained for the specimens treated in the highest temperature. In Table 1, the change of the effective refractive index was calculated by subtracting the effective index of thermally modified specimen from that of untreated one. This value is proposed to be proportional to the loss of birefringence of cellulose. We remark that similar result was obtained in the article of Degushi , where cellulose in water at temperature around 320°C and at constant pressure of 25 MPa was investigated. We suggest that the backscattering signal, measured with the MFS, yields information on the crystal to amorphous change of cellulose in the thermal modification process of wood. In Table 1 is presented density and also the relative change of the effective refractive index of the treated wood with respect to untreated one. This percentage is suggested to show the change of density/porosity of the treated wood sample. The thermally modified pine samples of this study had a lower density than the untreated pine which is assumed to result from changes of the sample mass during the heat treatment process when wood loses its weight . Naturally, for comprehensive statistical analysis the number of wood samples should be much higher than we measured because the density of the wood is a subject of variation not only among tree species but also among specimens of the same sample . The complexity of the density, porosity and pore size distribution of thermally treated spruce and maple has been investigated .
Further research is needed in order to verify the results with larger set of specimens and different tree species. However, this preliminary study indicates that the refractive index shows high potential for defining the degree of thermal modification after the treatment process.
In this paper, we have presented a light backscattering technique and a multifunction spectrophotometer to obtain effective refractive index for thermally modified Scots pine wood. Our measurements were based on the immersion liquid method. In this study, the wavelength was fixed. However, it is possible to freely choose the measurement wavelength of the light. This can have importance in basic studies of wood and wood products such as paper. In the case of paper the refractive index information is important in the aim of improving the opacity of the paper. We suggest that the immersion method and the MFS are useful in the basic studies of optical properties of thermally modified wood. Using the index data it is possible to assess changes in the porosity and crystalline forms of cellulose of thermally modified wood as a function of temperature and the treatment time. The proposed method will have importance in the quality inspection of thermally modified wood, and help to monitor and develop the industrial treatment process for thermal modification of wood.
- Thermowood® production statistics (2010) International Thermowood® Association. http://www.thermowood.fi. Accessed 5 May 2011
- Borrega M, Nevalainen S, Heräjärvi H (2009) Resistance of European and hybrid aspen wood against two brown-rot fungi. Holz als Roh- und Werkstoff 67(2):177–182View ArticleGoogle Scholar
- Hill CAS (2006) Wood modification: chemical thermal and other processes. Wiley, Chichester, p 239View ArticleGoogle Scholar
- Heräjärvi H (2009) Effect of drying technology on aspen wood properties. Silva Fenn 43(3):433–445Google Scholar
- Mitsui K, Inagaki T, Tsuchikawa S (2008) Monitoring of hydroxyl groups in wood during heat treatment using NIR spectroscopy. Biomacromolecules 9(1):286–288PubMedView ArticleGoogle Scholar
- Andersson S, Serimaa R, Väänänen T, Paakkari T, Jämsä S, Viitaniemi P (2005) X-ray scattering studies of thermally modified Scots pine (Pinus sylvestris L.). Holzforschung 59(4):422–427View ArticleGoogle Scholar
- Rowell RM (2005) Handbook of wood chemistry and wood composites. CRC Press, Boca Raton, FLGoogle Scholar
- Granston ED, Gray DG (2008) Birefringence in spin-coated films containing cellulose nanocrystals. Colloids Surface A 325:44–51View ArticleGoogle Scholar
- Winchell AN (1987) The optical properties of organic compounds, 2nd edn. Academic Press, ChicagoGoogle Scholar
- Saarela JMS, Heikkinen SM, Fabritius TEJ, Haapala AT, Myllylä RA (2008) Refractive index matching improves optical object detection in paper. Meas Sci Technol 19:1–7View ArticleGoogle Scholar
- Ye C (2007) Spectroscopic imaging ellipsometry of wood fiber cell walls: a comparison with confocal microscopy. Tappi J 6(8):26–32Google Scholar
- Page DH, El-Hosseiny F (1974) The birefringence and wood pulp fibres and the thickness of the S1 and S2 layers. Wood Fiber Sci 6:186–192Google Scholar
- Gindl W, Reifferscheid M, Adusmalli R-B, Weber H, Röder T, Sixta H, Schölberl T (2008) Anisotropy of the modulus of elasticity in regenerated cellulose fibres related to molecular orientation. Polymer 49:792–799View ArticleGoogle Scholar
- Peura M, Müller M, Serimaa R, Vainio U, Sarén M-P, Saranpää P, Burghammer M (2005) Structural studies of single wood cell walls by synchrotron X-ray microdiffraction and polarized light microscopy. Nucl Instr Methods Phys Res B 238:16–20View ArticleGoogle Scholar
- Sasaki Y, Hasegawa M (2007) Effect of anisotropy on acoustoelastic birefringence in wood. Ultrasonics 46:184–190PubMedView ArticleGoogle Scholar
- Reid M, Fedosejevs R (2006) Terahertz birefringence and attenuation properties of wood and paper. Appl Opt 45(12):2766–2772PubMedView ArticleGoogle Scholar
- Webster JG (1990) The measurement instrumentation and sensor handbook. CRC Press, FloridaGoogle Scholar
- Donaldson LA (1991) The use of pit apertures as windows to measure microfiber angle in chemical pulp fibers. Wood Fiber Sci 32:290–295Google Scholar
- Van Hilten D (1969) Refractive indices of minerals through the microscope: a similar method oblique observation. Am Mineral 66:549–553Google Scholar
- Marquis RE (1973) Immersion refractometry of isolated bacterial cell walls. J Bacteriol 116(3):1273–1279PubMedGoogle Scholar
- Papaev AV, Simonenko GV, Tuchin VV, Denisova TP (2006) Optical anisotropy of a biological tissue under conditions of immersion clearing and without them. Opt Spectrosc 101(1):46–53View ArticleGoogle Scholar
- Koivunen K, Niskanen I, Peiponen K-E, Paulapuro H (2009) Novel nanostructured PCC filters. J Mater Sci 44(2):477–482View ArticleGoogle Scholar
- Niskanen I, Räty J, Peiponen K-E (2008) Estimation of effective refractive index of birefringent particles using a combination of immersion liquid method and light scattering. Appl Spectrosc 62:399–401PubMedView ArticleGoogle Scholar
- Niskanen I, Räty J, Peiponen K-E (2010) Optical sensing of concentration and effective refractive index of pigments in a suspension. Appl Opt 49(17):3429–3433View ArticleGoogle Scholar
- ThermoWood Handbook (2003) Finnish Thermowood Association, Helsinki, FinlandGoogle Scholar
- Niskanen I, Räty J, Peiponen K-E (2006) A multifunction spectrophotometer for measurement of optical properties of transparent and turbid liquids. Meas Sci Technol 17:N87–N91View ArticleGoogle Scholar
- El-Hinnawi E–E (1966) Methods in chemical and mineral microscopy. Elsevier, Amsterdam, pp 36–37Google Scholar
- Weidler PG, Friedrich F (2007) Determination of the refractive index of particles in the clay and sub-micrometer size range. Am Mineral 92:1130–1132View ArticleGoogle Scholar
- Alén R, Kotilainen R, Zaman A (2002) Thermochemical behavior of Norway spruce (Picea abies) at 180–225°C. Wood Sci Technol 36:163–171View ArticleGoogle Scholar
- Yilldiz S, Gümüşkaya E (2007) The effects of thermal modification on crystalline structure of cellulose in soft and hardwood. Build Environ 42:62–67View ArticleGoogle Scholar
- Degushi S, Tsujii K, Horikoshi K (2006) Cooking cellulose in hot and compressed water. Chem Commun 31:3293–3295View ArticleGoogle Scholar
- Pfriem A, Zauer M, Wagenführ A (2009) Alteration of the pore structure of spruce (Picea abies (L.) Karst.) and maple (Acer pseudoplatanus L.) due to thermal treatment as determined by helium pycnometry and mercury intrusion porosimetry. Holzforschung 63:94–98View ArticleGoogle Scholar